Upcoming SlideShare
×

Capítulo 09 solda

295 views

Published on

projeto de engenharia shigley resolução

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total views
295
On SlideShare
0
From Embeds
0
Number of Embeds
3
Actions
Shares
0
8
0
Likes
0
Embeds 0
No embeds

No notes for slide

Capítulo 09 solda

1. 1. Chapter 9 9-1 Eq. (9-3): F = 0.707hlτ = 0.707(5/16)(4)(20) = 17.7 kip Ans. 9-2 Table 9-6: τall = 21.0 kpsi f = 14.85h kip/in = 14.85(5/16) = 4.64 kip/in F = f l = 4.64(4) = 18.56 kip Ans. 9-3 Table A-20: 1018 HR: Sut = 58 kpsi, Sy = 32 kpsi 1018 CR: Sut = 64 kpsi, Sy = 54 kpsi Cold-rolled properties degrade to hot-rolled properties in the neighborhood of the weld. Table 9-4: τall = min(0.30Sut, 0.40Sy) = min[0.30(58), 0.40(32)] = min(17.4, 12.8) = 12.8 kpsi for both materials. Eq. (9-3): F = 0.707hlτall F = 0.707(5/16)(4)(12.8) = 11.3 kip Ans. 9-4 Eq. (9-3) τ = √ 2F hl = √ 2(32) (5/16)(4)(2) = 18.1 kpsi Ans. 9-5 b = d = 2 in (a) Primary shear Table 9-1 τy = V A = F 1.414(5/16)(2) = 1.13F kpsi F 7" 1.414 shi20396_ch09.qxd 8/19/03 9:30 AM Page 246
2. 2. Chapter 9 247 Secondary shear Table 9-1 Ju = d(3b2 + d2) 6 = 2[(3)(22) + 22] 6 = 5.333 in3 J = 0.707hJu = 0.707(5/16)(5.333) = 1.18 in4 τx = τy = Mry J = 7F(1) 1.18 = 5.93F kpsi Maximum shear τmax = τ 2 x + (τy + τy )2 = F 5.932 + (1.13 + 5.93)2 = 9.22F kpsi F = τall 9.22 = 20 9.22 = 2.17 kip Ans. (1) (b) For E7010 from Table 9-6, τall = 21 kpsi Table A-20: HR 1020 Bar: Sut = 55 kpsi, Sy = 30 kpsi HR 1015 Support: Sut = 50 kpsi, Sy = 27.5 kpsi Table 9-5, E7010 Electrode: Sut = 70 kpsi, Sy = 57 kpsi Therefore, the bar controls the design. Table 9-4: τall = min[0.30(50), 0.40(27.5)] = min[15, 11] = 11 kpsi The allowable load from Eq. (1) is F = τall 9.22 = 11 9.22 = 1.19 kip Ans. 9-6 b = d = 2 in Primary shear τy = V A = F 4(0.707)(5/16)(2) = 0.566F Secondary shear Table 9-1: Ju = (b + d)3 6 = (2 + 2)3 6 = 10.67 in3 J = 0.707hJu = 0.707(5/16)(10.67) = 2.36 in4 τx = τy = Mry J = (7F)(1) 2.36 = 2.97F F 7" shi20396_ch09.qxd 8/19/03 9:30 AM Page 247
3. 3. 248 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design Maximum shear τmax = τ 2 x + (τy + τy )2 = F 2.972 + (0.556 + 2.97)2 = 4.61F kpsi F = τall 4.61 Ans. which is twice τmax/9.22 of Prob. 9-5. 9-7 Weldment, subjected to alternating fatigue, has throat area of A = 0.707(6)(60 + 50 + 60) = 721 mm2 Members’endurance limit: AISI 1010 steel Sut = 320 MPa, Se = 0.504(320) = 161.3 MPa ka = 272(320)−0.995 = 0.875 kb = 1 (direct shear) kc = 0.59 (shear) kd = 1 kf = 1 Kf s = 1 2.7 = 0.370 Sse = 0.875(1)(0.59)(0.37)(161.3) = 30.81 MPa Electrode’s endurance: 6010 Sut = 62(6.89) = 427 MPa Se = 0.504(427) = 215 MPa ka = 272(427)−0.995 = 0.657 kb = 1 (direct shear) kc = 0.59 (shear) kd = 1 kf = 1/Kf s = 1/2.7 = 0.370 Sse = 0.657(1)(0.59)(0.37)(215) = 30.84 MPa . = 30.81 Thus, the members and the electrode are of equal strength. For a factor of safety of 1, Fa = τa A = 30.8(721)(10−3 ) = 22.2 kN Ans. shi20396_ch09.qxd 8/19/03 9:30 AM Page 248
4. 4. Chapter 9 249 9-8 Primary shear τ = 0 (why?) Secondary shear Table 9-1: Ju = 2πr3 = 2π(4)3 = 402 cm3 J = 0.707hJu = 0.707(0.5)(402) = 142 cm4 M = 200F N · m (F in kN) τ = Mr 2J = (200F)(4) 2(142) = 2.82F (2 welds) F = τall τ = 140 2.82 = 49.2 kN Ans. 9-9 Rank fom = Ju lh = a3 /12 ah = a2 12h = 0.0833 a2 h 5 fom = a(3a2 + a2 ) 6(2a)h = a2 3h = 0.3333 a2 h 1 fom = (2a)4 − 6a2 a2 12(a + a)2ah = 5a2 24h = 0.2083 a2 h 4 fom = 1 3ah 8a3 + 6a3 + a3 12 − a4 2a + a = 11 36 a2 h = 0.3056 a2 h 2 fom = (2a)3 6h 1 4a = 8a3 24ah = a2 3h = 0.3333 a2 h 1 fom = 2π(a/2)3 πah = a3 4ah = a2 4h = 0.25 a2 h 3 These rankings apply to ﬁllet weld patterns in torsion that have a square area a × a in which to place weld metal. The object is to place as much metal as possible to the border. If your area is rectangular, your goal is the same but the rankings may change. Students will be surprised that the circular weld bead does not rank ﬁrst. 9-10 fom = Iu lh = 1 a a3 12 1 h = 1 12 a2 h = 0.0833 a2 h 5 fom = Iu lh = 1 2ah a3 6 = 0.0833 a2 h 5 fom = Iu lh = 1 2ah a2 2 = 1 4 a2 h = 0.25 a2 h 1 shi20396_ch09.qxd 8/19/03 9:30 AM Page 249
5. 5. 250 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design fom = Iu lh = 1 [2(2a)]h a2 6 (3a + a) = 1 6 a2 h = 0.1667 a2 h 2 ¯x = b 2 = a 2 , ¯y = d2 b + 2d = a2 3a = a 3 Iu = 2d3 3 − 2d2 a 3 + (b + 2d) a2 9 = 2a3 3 − 2a3 3 + 3a a2 9 = a3 3 fom = Iu lh = a3 /3 3ah = 1 9 a2 h = 0.1111 a2 h 4 Iu = πr3 = πa3 8 fom = Iu lh = πa3 /8 πah = a2 8h = 0.125 a2 h 3 The CEE-section pattern was not ranked because the deﬂection of the beam is out-of-plane. If you have a square area in which to place a ﬁllet weldment pattern under bending, your objective is to place as much material as possible away from the x-axis. If your area is rec- tangular, your goal is the same, but the rankings may change. 9-11 Materials: Attachment (1018 HR) Sy = 32 kpsi, Sut = 58 kpsi Member (A36) Sy = 36 kpsi, Sut ranges from 58 to 80 kpsi, use 58. The member and attachment are weak compared to the E60XX electrode. Decision Specify E6010 electrode Controlling property: τall = min[0.3(58), 0.4(32)] = min(16.6, 12.8) = 12.8 kpsi For a static load the parallel and transverse ﬁllets are the same. If n is the number of beads, τ = F n(0.707)hl = τall nh = F 0.707lτall = 25 0.707(3)(12.8) = 0.921 Make a table. Number of beads Leg size n h 1 0.921 2 0.460 →1/2" 3 0.307 →5/16" 4 0.230 →1/4" Decision: Specify 1/4" leg size Decision: Weld all-around shi20396_ch09.qxd 8/19/03 9:30 AM Page 250
6. 6. Chapter 9 251 Weldment Speciﬁcations: Pattern: All-around square Electrode: E6010 Type: Two parallel ﬁllets Ans. Two transverse ﬁllets Length of bead: 12 in Leg: 1/4 in For a ﬁgure of merit of, in terms of weldbead volume, is this design optimal? 9-12 Decision: Choose a parallel ﬁllet weldment pattern. By so-doing, we’ve chosen an optimal pattern (see Prob. 9-9) and have thus reduced a synthesis problem to an analysis problem: Table 9-1: A = 1.414hd = 1.414(h)(3) = 4.24h in3 Primary shear τy = V A = 3000 4.24h = 707 h Secondary shear Table 9-1: Ju = d(3b2 + d2 ) 6 = 3[3(32 ) + 32 ] 6 = 18 in3 J = 0.707(h)(18) = 12.7h in4 τx = Mry J = 3000(7.5)(1.5) 12.7h = 2657 h = τy τmax = τ 2 x + (τy + τy )2 = 1 h 26572 + (707 + 2657)2 = 4287 h Attachment (1018 HR): Sy = 32 kpsi, Sut = 58 kpsi Member (A36): Sy = 36 kpsi The attachment is weaker Decision: Use E60XX electrode τall = min[0.3(58), 0.4(32)] = 12.8 kpsi τmax = τall = 4287 h = 12 800 psi h = 4287 12 800 = 0.335 in Decision: Specify 3/8" leg size Weldment Speciﬁcations: Pattern: Parallel ﬁllet welds Electrode: E6010 Type: Fillet Ans. Length of bead: 6 in Leg size: 3/8 in shi20396_ch09.qxd 8/19/03 9:30 AM Page 251
7. 7. 252 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design 9-13 An optimal square space (3" × 3") weldment pattern is ԽԽ or or ᮀ. In Prob. 9-12, there was roundup of leg size to3/8 in. Consider the member material to be structural A36 steel. Decision: Use a parallel horizontal weld bead pattern for welding optimization and convenience. Materials: Attachment (1018 HR): Sy = 32 kpsi, Sut = 58 kpsi Member (A36): Sy = 36 kpsi, Sut 58–80 kpsi; use 58 kpsi From Table 9-4 AISC welding code, τall = min[0.3(58), 0.4(32)] = min(16.6, 12.8) = 12.8 kpsi Select a stronger electrode material from Table 9-3. Decision: Specify E6010 Throat area and other properties: A = 1.414hd = 1.414(h)(3) = 4.24h in2 ¯x = b/2 = 3/2 = 1.5 in ¯y = d/2 = 3/2 = 1.5 in Ju = d(3b2 + d2 ) 6 = 3[3(32 ) + 32 ] 6 = 18 in3 J = 0.707hJu = 0.707(h)(18) = 12.73h in4 Primary shear: τx = V A = 3000 4.24h = 707.5 h Secondary shear: τ = Mr J τx = τ cos 45◦ = Mr J cos 45◦ = Mrx J τx = 3000(6 + 1.5)(1.5) 12.73h = 2651 h τy = τx = 2651 h ry x rx r ␶ЈЈ ␶ЈЈ ␶Ј y x x ␶ЈЈy shi20396_ch09.qxd 8/19/03 9:30 AM Page 252
8. 8. Chapter 9 253 τmax = (τx + τx)2 + τ 2 y = 1 h (2651 + 707.5)2 + 26512 = 4279 h psi Relate stress and strength: τmax = τall 4279 h = 12 800 h = 4279 12 800 = 0.334 in → 3/8 in Weldment Speciﬁcations: Pattern: Horizontal parallel weld tracks Electrode: E6010 Type of weld: Two parallel ﬁllet welds Length of bead: 6 in Leg size: 3/8 in Additional thoughts: Since the round-up in leg size was substantial, why not investigate a backward C weld pattern. One might then expect shorter horizontal weld beads which will have the advan- tage of allowing a shorter member (assuming the member has not yet been designed). This will show the inter-relationship between attachment design and supporting members. 9-14 Materials: Member (A36): Sy = 36 kpsi, Sut = 58 to 80 kpsi; use Sut = 58 kpsi Attachment (1018 HR): Sy = 32 kpsi, Sut = 58 kpsi τall = min[0.3(58), 0.4(32)] = 12.8 kpsi Decision: Use E6010 electrode. From Table 9-3: Sy = 50 kpsi, Sut = 62 kpsi, τall = min[0.3(62), 0.4(50)] = 20 kpsi Decision: Since A36 and 1018 HR are weld metals to an unknown extent, use τall = 12.8 kpsi Decision: Usethemostefﬁcientweldpattern–square,weld-all-around.Choose6" × 6" size. Attachment length: l1 = 6 + a = 6 + 6.25 = 12.25 in Throat area and other properties: A = 1.414h(b + d) = 1.414(h)(6 + 6) = 17.0h ¯x = b 2 = 6 2 = 3 in, ¯y = d 2 = 6 2 = 3 in shi20396_ch09.qxd 8/19/03 9:30 AM Page 253
9. 9. 254 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design Primary shear τy = V A = F A = 20 000 17h = 1176 h psi Secondary shear Ju = (b + d)3 6 = (6 + 6)3 6 = 288 in3 J = 0.707h(288) = 203.6h in4 τx = τy = Mry J = 20 000(6.25 + 3)(3) 203.6h = 2726 h psi τmax = τ 2 x + (τy + τy)2 = 1 h 27262 + (2726 + 1176)2 = 4760 h psi Relate stress to strength τmax = τall 4760 h = 12 800 h = 4760 12 800 = 0.372 in Decision: Specify 3/8 in leg size Speciﬁcations: Pattern: All-around square weld bead track Electrode: E6010 Type of weld: Fillet Weld bead length: 24 in Leg size: 3/8 in Attachment length: 12.25 in 9-15 This is a good analysis task to test the students’ understanding (1) Solicit information related to a priori decisions. (2) Solicit design variables b and d. (3) Find h and round and output all parameters on a single screen. Allow return to Step 1 or Step 2 (4) When the iteration is complete, the ﬁnal display can be the bulk of your adequacy assessment. Such a program can teach too. 9-16 The objective of this design task is to have the students teach themselves that the weld patterns of Table 9-3 can be added or subtracted to obtain the properties of a comtem- plated weld pattern. The instructor can control the level of complication. I have left the shi20396_ch09.qxd 8/19/03 9:30 AM Page 254
10. 10. Chapter 9 255 presentation of the drawing to you. Here is one possibility. Study the problem’s opportuni- ties, then present this (or your sketch) with the problem assignment. Use b1 as the design variable. Express properties as a function of b1 . From Table 9-3, category 3: A = 1.414h(b − b1) ¯x = b/2, ¯y = d/2 Iu = bd2 2 − b1d2 2 = (b − b1)d2 2 I = 0.707hIu τ = V A = F 1.414h(b − b1) τ = Mc I = Fa(d/2) 0.707hIu τmax = τ 2 + τ 2 Parametric study Let a = 10 in, b = 8 in, d = 8 in, b1 = 2 in, τall = 12.8 kpsi, l = 2(8 − 2) = 12 in A = 1.414h(8 − 2) = 8.48h in2 Iu = (8 − 2)(82 /2) = 192 in3 I = 0.707(h)(192) = 135.7h in4 τ = 10 000 8.48h = 1179 h psi τ = 10 000(10)(8/2) 135.7h = 2948 h psi τmax = 1 h 11792 + 29482 = 3175 h = 12 800 from which h = 0.248 in. Do not round off the leg size – something to learn. fom = Iu hl = 192 0.248(12) = 64.5 A = 8.48(0.248) = 2.10 in2 I = 135.7(0.248) = 33.65 in4 Section AA A36 Body welds not shown 8" 8" 1 2 " a A A 10000 lbf 1018 HR Attachment weld pattern considered b b1 d shi20396_ch09.qxd 8/19/03 9:30 AM Page 255
11. 11. 256 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design vol = h2 2 l = 0.2482 2 12 = 0.369 in3 I vol = 33.65 0.369 = 91.2 = eff τ = 1179 0.248 = 4754 psi τ = 2948 0.248 = 11 887 psi τmax = 4127 0.248 . = 12 800 psi Now consider the case of uninterrupted welds, b1 = 0 A = 1.414(h)(8 − 0) = 11.31h Iu = (8 − 0)(82 /2) = 256 in3 I = 0.707(256)h = 181h in4 τ = 10 000 11.31h = 884 h τ = 10 000(10)(8/2) 181h = 2210 h τmax = 1 h 8842 + 22102 = 2380 h = τall h = τmax τall = 2380 12 800 = 0.186 in Do not round off h. A = 11.31(0.186) = 2.10 in2 I = 181(0.186) = 33.67 τ = 884 0.186 = 4753 psi, vol = 0.1862 2 16 = 0.277 in3 τ = 2210 0.186 = 11 882 psi fom = Iu hl = 256 0.186(16) = 86.0 eff = I (h2/2)l = 33.67 (0.1862/2)16 = 121.7 Conclusions: To meet allowable stress limitations, I and A do not change, nor do τ and σ. To meet the shortened bead length, h is increased proportionately. However, volume of bead laid down increases as h2 . The uninterrupted bead is superior. In this example, we did not round h and as a result we learned something. Our measures of merit are also sensitive to rounding. When the design decision is made, rounding to the next larger standard weld ﬁllet size will decrease the merit. shi20396_ch09.qxd 8/19/03 9:30 AM Page 256
12. 12. Chapter 9 257 Had the weld bead gone around the corners, the situation would change. Here is a fol- lowup task analyzing an alternative weld pattern. 9-17 From Table 9-2 For the box A = 1.414h(b + d) Subtracting b1 from b and d1 from d A = 1.414 h(b − b1 + d − d1) Iu = d2 6 (3b + d) − d3 1 6 − b1d2 2 = 1 2 (b − b1)d2 + 1 6 d3 − d3 1 length of bead l = 2(b − b1 + d − d1) fom = Iu/hl 9-18 Below is a Fortran interactive program listing which, if imitated in any computer language of convenience, will reduce to drudgery. Furthermore, the program allows synthesis by in- teraction or learning without fatigue. C Weld2.f for rect. fillet beads resisting bending C. Mischke Oct 98 1 print*,’weld2.f rectangular fillet weld-beads in bending,’ print*,’gaps allowed - C. Mischke Oct. 98’ print*,’ ’ print*,’Enter largest permissible shear stress tauall’ read*,tauall print*,’Enter force F and clearance a’ read*,F,a 2 print*,’Enter width b and depth d of rectangular pattern’ read*,b,d xbar=b/2. ybar=d/2. 3 print*,’Enter width of gap b1, and depth of gap d1’ print*,’both gaps central in their respective sides’ read*,b1,d1 xIu=(b-b1)*d**2/2.+(d**3-d1**3)/6. xl=2.*(d-d1)+2.*(b-b1) b b1 dd1 shi20396_ch09.qxd 8/19/03 9:30 AM Page 257
13. 13. 258 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design C Following calculations based on unit leg h = 1 AA=1.414*(b-b1+d-d1) xI=0.707*xIu tau2=F*a*d/2./xI tau1=F/AA taumax=sqrt(tau2**2+tau1**2) h=taumax/tauall C Adjust parameters for now-known h AA=AA*h xI=xI*h tau2=tau2/h tau1=tau1/h taumax=taumax/h fom=xIu/h/xl print*,’F=’,F,’ a=’,a,’ bead length = ’,xl print*,’b=’,b,’ b1=’,b1,’ d=’,d,’ d1=’,d1 print*,’xbar=’,xbar,’ ybar=’,ybar,’ Iu=’,xIu print*,’I=’,xI,’ tau2=’,tau2,’ tau1=’,tau1 print*,’taumax=’,taumax,’ h=’,h,’ A=’,AA print*,’fom=’,fom, ’I/(weld volume)=’,2.*xI/h**2/xl print*,’ ’ print*,’To change b1,d1: 1; b,d: 2; New: 3; Quit: 4’ read*,index go to (3,2,1,4), index 4 call exit end 9-19 τall = 12 800 psi. Use Fig. 9-17(a) for general geometry, but employ beads and then ԽԽ beads. Horizontal parallel weld bead pattern b = 6 in d = 8 in From Table 9-2, category 3 A = 1.414 hb = 1.414(h)(6) = 8.48 h in2 ¯x = b/2 = 6/2 = 3 in, ¯y = d/2 = 8/2 = 4 in Iu = bd2 2 = 6(8)2 2 = 192 in3 I = 0.707hIu = 0.707(h)(192) = 135.7h in4 τ = 10 000 8.48h = 1179 h psi 6" 8" shi20396_ch09.qxd 8/19/03 9:30 AM Page 258
14. 14. Chapter 9 259 τ = Mc I = 10 000(10)(8/2) 135.7h = 2948 h psi τmax = τ 2 + τ 2 = 1 h (11792 + 29482 )1/2 = 3175 h psi Equate the maximum and allowable shear stresses. τmax = τall = 3175 h = 12 800 from which h = 0.248 in. It follows that I = 135.7(0.248) = 33.65 in4 The volume of the weld metal is vol = h2 l 2 = 0.2482 (6 + 6) 2 = 0.369 in3 The effectiveness, (eff)H , is (eff)H = I vol = 33.65 0.369 = 91.2 in (fom )H = Iu hl = 192 0.248(6 + 6) = 64.5 in Vertical parallel weld beads b = 6 in d = 8 in From Table 9-2, category 2 A = 1.414hd = 1.414(h)(8) = 11.31h in2 ¯x = b/2 = 6/2 = 3 in, ¯y = d/2 = 8/2 = 4 in Iu = d3 6 = 83 6 = 85.33 in3 I = 0.707hIu = 0.707(h)(85.33) = 60.3h τ = 10 000 11.31h = 884 h psi τ = Mc I = 10 000(10)(8/2) 60.3 h = 6633 h psi τmax = τ 2 + τ 2 = 1 h (8842 + 66332 )1/2 = 6692 h psi 8" 6" shi20396_ch09.qxd 8/19/03 9:30 AM Page 259
15. 15. 260 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design Equating τmax to τall gives h = 0.523 in. It follows that I = 60.3(0.523) = 31.5 in4 vol = h2 l 2 = 0.5232 2 (8 + 8) = 2.19 in3 (eff)V = I vol = 31.6 2.19 = 14.4 in (fom )V = Iu hl = 85.33 0.523(8 + 8) = 10.2 in The ratio of (eff)V/(eff)H is 14.4/91.2 = 0.158. The ratio (fom )V/(fom )H is 10.2/64.5 = 0.158. This is not surprising since eff = I vol = I (h2/2)l = 0.707 hIu (h2/2)l = 1.414 Iu hl = 1.414 fom The ratios (eff)V/(eff)H and (fom )V/(fom )H give the same information. 9-20 Because the loading is pure torsion, there is no primary shear. From Table 9-1, category 6: Ju = 2πr3 = 2π(1)3 = 6.28 in3 J = 0.707 hJu = 0.707(0.25)(6.28) = 1.11 in4 τ = Tr J = 20(1) 1.11 = 18.0 kpsi Ans. 9-21 h = 0.375 in, d = 8 in, b = 1 in From Table 9-2, category 2: A = 1.414(0.375)(8) = 4.24 in2 Iu = d3 6 = 83 6 = 85.3 in3 I = 0.707hIu = 0.707(0.375)(85.3) = 22.6 in4 τ = F A = 5 4.24 = 1.18 kpsi M = 5(6) = 30 kip · in c = (1 + 8 + 1 − 2)/2 = 4 in τ = Mc I = 30(4) 22.6 = 5.31 kpsi τmax = τ 2 + τ 2 = 1.182 + 5.312 = 5.44 kpsi Ans. shi20396_ch09.qxd 8/19/03 9:30 AM Page 260
16. 16. Chapter 9 261 9-22 h = 0.6 cm, b = 6 cm, d = 12 cm. Table 9-3, category 5: A = 0.707h(b + 2d) = 0.707(0.6)[6 + 2(12)] = 12.7 cm2 ¯y = d2 b + 2d = 122 6 + 2(12) = 4.8 cm Iu = 2d3 3 − 2d2 ¯y + (b + 2d) ¯y2 = 2(12)3 3 − 2(122 )(4.8) + [6 + 2(12)]4.82 = 461 cm3 I = 0.707hIu = 0.707(0.6)(461) = 196 cm4 τ = F A = 7.5(103) 12.7(102) = 5.91 MPa M = 7.5(120) = 900 N · m cA = 7.2 cm, cB = 4.8 cm The critical location is at A. τA = McA I = 900(7.2) 196 = 33.1 MPa τmax = τ 2 + τ 2 = (5.912 + 33.12 )1/2 = 33.6 MPa n = τall τmax = 120 33.6 = 3.57 Ans. 9-23 The largest possible weld size is 1/16 in. This is a small weld and thus difﬁcult to accom- plish. The bracket’s load-carrying capability is not known. There are geometry problems associated with sheet metal folding, load-placement and location of the center of twist. This is not available to us. We will identify the strongest possible weldment. Use a rectangular, weld-all-around pattern – Table 9-2, category 6: A = 1.414 h(b + d) = 1.414(1/16)(1 + 7.5) = 0.751 in2 ¯x = b/2 = 0.5 in ¯y = d 2 = 7.5 2 = 3.75 in 6 4.8 7.2 A B G 1" 7.5" shi20396_ch09.qxd 8/19/03 9:30 AM Page 261
17. 17. 262 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design Iu = d2 6 (3b + d) = 7.52 6 [3(1) + 7.5] = 98.4 in3 I = 0.707hIu = 0.707(1/16)(98.4) = 4.35 in4 M = (3.75 + 0.5)W = 4.25W τ = V A = W 0.751 = 1.332W τ = Mc I = 4.25W(7.5/2) 4.35 = 3.664W τmax = τ 2 + τ 2 = W 1.3322 + 3.6642 = 3.90W Material properties: The allowable stress given is low. Let’s demonstrate that. For the A36 structural steel member, Sy = 36 kpsi and Sut = 58 kpsi. For the 1020 CD attachment, use HR properties of Sy = 30 kpsi and Sut = 55. The E6010 electrode has strengths of Sy = 50 and Sut = 62 kpsi. Allowable stresses: A36: τall = min[0.3(58), 0.4(36)] = min(17.4, 14.4) = 14.4 kpsi 1020: τall = min[0.3(55), 0.4(30)] τall = min(16.5, 12) = 12 kpsi E6010: τall = min[0.3(62), 0.4(50)] = min(18.6, 20) = 18.6 kpsi Since Table 9-6 gives 18.0 kpsi as the allowable shear stress, use this lower value. Therefore, the allowable shear stress is τall = min(14.4, 12, 18.0) = 12 kpsi However, the allowable stress in the problem statement is 0.9 kpsi which is low from the weldment perspective. The load associated with this strength is τmax = τall = 3.90W = 900 W = 900 3.90 = 231 lbf If the welding can be accomplished (1/16 leg size is a small weld), the weld strength is 12 000 psi and the load W = 3047 lbf. Can the bracket carry such a load? There are geometry problems associated with sheet metal folding. Load placement is important and the center of twist has not been identiﬁed. Also, the load-carrying capability of the top bend is unknown. These uncertainties may require the use of a different weld pattern. Our solution pro- vides the best weldment and thus insight for comparing a welded joint to one which em- ploys screw fasteners. shi20396_ch09.qxd 8/19/03 9:30 AM Page 262
18. 18. Chapter 9 263 9-24 F = 100 lbf, τall = 3 kpsi FB = 100(16/3) = 533.3 lbf Fx B = −533.3 cos 60◦ = −266.7 lbf F y B = −533.3 cos 30◦ = −462 lbf It follows that R y A = 562 lbf and Rx A = 266.7 lbf, RA = 622 lbf M = 100(16) = 1600 lbf · in The OD of the tubes is 1 in. From Table 9-1, category 6: A = 1.414(πhr)(2) = 2(1.414)(πh)(1/2) = 4.44h in2 Ju = 2πr3 = 2π(1/2)3 = 0.785 in3 J = 2(0.707)hJu = 1.414(0.785)h = 1.11h in4 τ = V A = 622 4.44h = 140 h τ = Tc J = Mc J = 1600(0.5) 1.11h = 720.7 h The shear stresses, τ and τ , are additive algebraically τmax = 1 h (140 + 720.7) = 861 h psi τmax = τall = 861 h = 3000 h = 861 3000 = 0.287 → 5/16" Decision: Use 5/16 in ﬁllet welds Ans. 100 16 3 562 266.7 266.7 462 F FB B A R x A R y A 60Њ y x shi20396_ch09.qxd 8/19/03 9:30 AM Page 263
19. 19. 264 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design 9-25 For the pattern in bending shown, ﬁnd the centroid G of the weld group. ¯x = 6(0.707)(1/4)(3) + 6(0.707)(3/8)(13) 6(0.707)(1/4) + 6(0.707)(3/8) = 9 in I1/4 = 2 IG + A2 ¯x = 2 0.707(1/4)(63 ) 12 + 0.707(1/4)(6)(62 ) = 82.7 in4 I3/8 = 2 0.707(3/8)(63 ) 12 + 0.707(3/8)(6)(42 ) = 60.4 in4 I = I1/4 + I3/8 = 82.7 + 60.4 = 143.1 in4 The critical location is at B. From Eq. (9-3), τ = F 2[6(0.707)(3/8 + 1/4)] = 0.189F τ = Mc I = (8F)(9) 143.1 = 0.503F τmax = τ 2 + τ 2 = F 0.1892 + 0.5032 = 0.537F Materials: A36 Member: Sy = 36 kpsi 1015 HR Attachment: Sy = 27.5 kpsi E6010 Electrode: Sy = 50 kpsi τall = 0.577 min(36, 27.5, 50) = 15.9 kpsi F = τall/n 0.537 = 15.9/2 0.537 = 14.8 kip Ans. 9-26 Figure P9-26b is a free-body diagram of the bracket. Forces and moments that act on the welds are equal, but of opposite sense. (a) M = 1200(0.366) = 439 lbf · in Ans. (b) Fy = 1200 sin 30◦ = 600 lbf Ans. (c) Fx = 1200 cos 30◦ = 1039 lbf Ans. 3 8 " 3 8 " 1 4 " 1 4 " 7"9" g g g g y x G B shi20396_ch09.qxd 8/19/03 9:30 AM Page 264
20. 20. Chapter 9 265 (d) From Table 9-2, category 6: A = 1.414(0.25)(0.25 + 2.5) = 0.972 in2 Iu = d2 6 (3b + d) = 2.52 6 [3(0.25) + 2.5] = 3.39 in3 The second area moment about an axis through G and parallel to z is I = 0.707hIu = 0.707(0.25)(3.39) = 0.599 in4 Ans. (e) Refer to Fig. P.9-26b. The shear stress due to Fy is τ1 = Fy A = 600 0.972 = 617 psi The shear stress along the throat due to Fx is τ2 = Fx A = 1039 0.972 = 1069 psi The resultant of τ1 and τ2 is in the throat plane τ = τ2 1 + τ2 2 1/2 = (6172 + 10692 )1/2 = 1234 psi The bending of the throat gives τ = Mc I = 439(1.25) 0.599 = 916 psi The maximum shear stress is τmax = (τ 2 + τ 2 )1/2 = (12342 + 9162 )1/2 = 1537 psi Ans. (f) Materials: 1018 HR Member: Sy = 32 kpsi, Sut = 58 kpsi (Table A-20) E6010 Electrode: Sy = 50 kpsi (Table 9-3) n = Ssy τmax = 0.577Sy τmax = 0.577(32) 1.537 = 12.0 Ans. (g) Bending in the attachment near the base. The cross-sectional area is approximately equal to bh. A1 . = bh = 0.25(2.5) = 0.625 in2 τxy = Fx A1 = 1039 0.625 = 1662 psi I c = bd2 6 = 0.25(2.5)2 6 = 0.260 in3 At location A σy = Fy A1 + M I/c σy = 600 0.625 + 439 0.260 = 2648 psi shi20396_ch09.qxd 8/19/03 9:30 AM Page 265
21. 21. 266 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design The von Mises stress σ is σ = σ2 y + 3τ2 xy 1/2 = [26482 + 3(1662)2 ]1/2 = 3912 psi Thus, the factor of safety is, n = Sy σ = 32 3.912 = 8.18 Ans. The clip on the mooring line bears against the side of the 1/2-in hole. If the clip ﬁlls the hole σ = F td = −1200 0.25(0.50) = −9600 psi n = − Sy σ = − 32(103 ) −9600 = 3.33 Ans. Further investigation of this situation requires more detail than is included in the task statement. (h) In shear fatigue, the weakest constituent of the weld melt is 1018 with Sut = 58 kpsi Se = 0.504Sut = 0.504(58) = 29.2 kpsi Table 7-4: ka = 14.4(58)−0.718 = 0.780 For the size factor estimate, we ﬁrst employ Eq. (7-24) for the equivalent diameter. de = 0.808 √ 0.707hb = 0.808 0.707(2.5)(0.25) = 0.537 in Eq. (7-19) is used next to ﬁnd kb kb = de 0.30 −0.107 = 0.537 0.30 −0.107 = 0.940 The load factor for shear kc , is kc = 0.59 The endurance strength in shear is Sse = 0.780(0.940)(0.59)(29.2) = 12.6 kpsi From Table 9-5, the shear stress-concentration factor is Kf s = 2.7. The loading is repeatedly-applied. τa = τm = kf τmax 2 = 2.7 1.537 2 = 2.07 kpsi Table 7-10: Gerber factor of safety nf , adjusted for shear, with Ssu = 0.67Sut nf = 1 2 0.67(58) 2.07 2 2.07 12.6    −1 + 1 + 2(2.07)(12.6) 0.67(58)(2.07) 2    = 5.55 Ans. Attachment metal should be checked for bending fatigue. shi20396_ch09.qxd 8/19/03 9:30 AM Page 266
22. 22. Chapter 9 267 9-27 Use b = d = 4 in. Since h = 5/8 in, the primary shear is τ = F 1.414(5/8)(4) = 0.283F The secondary shear calculations, for a moment arm of 14 in give Ju = 4[3(42 ) + 42 ] 6 = 42.67 in3 J = 0.707hJu = 0.707(5/8)42.67 = 18.9 in4 τx = τy = Mry J = 14F(2) 18.9 = 1.48F Thus, the maximum shear and allowable load are: τmax = F 1.482 + (0.283 + 1.48)2 = 2.30F F = τall 2.30 = 20 2.30 = 8.70 kip Ans. From Prob. 9-5b, τall = 11 kpsi Fall = τall 2.30 = 11 2.30 = 4.78 kip The allowable load has thus increased by a factor of 1.8 Ans. 9-28 Purchase the hook having the design shown in Fig. P9-28b. Referring to text Fig. 9-32a, this design reduces peel stresses. 9-29 (a) ¯τ = 1 l l/2 −l/2 Pω cosh(ωx) 4b sinh(ωl/2) dx = A1 l/2 −l/2 cosh(ωx) dx = A1 ω sinh(ωx) l/2 −l/2 = A1 ω [sinh(ωl/2) − sinh(−ωl/2)] = A1 ω [sinh(ωl/2) − (−sinh(ωl/2))] = 2A1 sinh(ωl/2) ω = Pω 4bl sinh(ωl/2) [2 sinh(ωl/2)] ¯τ = P 2bl Ans. shi20396_ch09.qxd 8/19/03 9:30 AM Page 267
23. 23. 268 Solutions Manual • Instructor’s Solution Manual to Accompany Mechanical Engineering Design (b) τ(l/2) = Pω cosh(ωl/2) 4b sinh(ωl/2) = Pω 4b tanh(ωl/2) Ans. (c) K = τ(l/2) ¯τ = Pω 4b sinh(ωl/2) 2bl P K = ωl/2 tanh(ωl/2) Ans. For computer programming, it can be useful to express the hyperbolic tangent in terms of exponentials: K = ωl 2 exp(ωl/2) − exp(−ωl/2) exp(ωl/2) + exp(−ωl/2) Ans. 9-30 This is a computer programming exercise. All programs will vary. shi20396_ch09.qxd 8/19/03 9:30 AM Page 268